Cement is the substance which holds concrete together, which means that
it is extremely widely used in our society. It has been manufactured in New
Zealand for more than 100 years, and during this century production has
increased one hundred-fold. Portland cement (the only type of cement in
common use today) is manufactured in a four step process.
Step 1 - Quarrying Limestone and a 'cement rock' such as clay or shale are
quarried and brought to the cement works. These rocks contain lime (CaCO3),
silica (SiO2), alumina (Al2O3) and ferrous oxide (Fe2O3) - the raw materials of
Step 2 - Raw material preparation To form a consistent product, it is essential that
the same mixture of minerals is used every time. For this reason the exact
composition of the limestone and clay is determined at this point, and other
ingredients added if necessary. The rock is also ground into fine particles to
increase the efficiency of the reaction.
Step 3 - Clinkering The raw materials are then dried, heated and fed into a
rotating kiln. Here the raw materials react at very high temperatures to form
3CaO• SiO2 (tricalcium silicate), 2CaO• SiO2 (dicalcium silicate), 3CaO• Al2O3
(tricalcium aluminate) and 4CaO• Al2O3 • Fe2O3 (tetracalcium alumino-ferrate).
Step 4 - Cement milling The 'clinker' that has now been produced will
behave just like cement, but it is in particles up to 3 cm in diameter. These
are ground down to a fine powder to turn the clinker into useful cement.
Cement production has several quite serious environmental hazards
associated with it: dust and CO2 emissions and contaminated run-off water.
Both cement works in New Zealand have measures in place to minimize
Concrete is an extremely versatile material, being used in the production of anything from
nuclear radiation shields to playground structures and from bridges to yachts. It is able to be
used in such a wide variety of applications because it can be poured into any shape,
reinforced with steel or glass fibers, precast, colored, has a variety of finishes and can even
set under water. Modern concrete is made by mixing aggregate (sand, stones and shingle)
with Portland cement and water and allowing it to set. Of these ingredients, the most
important is Portland cement. Cement is a fine grey powder which when reacted with water
hardens to form a rigid chemical mineral structure which gives concrete its high strengths.
Cement is in effect the glue that holds concrete together. The credit for its discovery is given
to the Romans, who mixed lime (CaCO3) with volcanic ash, producing a cement mortar which
was used during
construction of such impressive structures as the Colosseum. When the Roman empire fell, the information on
how to make cement was lost and was not rediscovered until the 16th century. A brief history of Portland
cement Cement has been made since Roman times, but over time the recipes used to make cement have been
refined. The earliest cements were made from lime and pozzolana (a volcanic ash containing significant
quantities of SiO2 and Al2O3) mixed with ground brick and water. This cement was not improved upon until
1758, when Smeaton noticed that using a limestone that was 20 - 25 % clay and heating the mixture resulted in a
cement that could harden under water. He called this new cement 'hydraulic lime'. When the mixture was
heated, a small quantity of it was sintered1 . Normally this was discarded as waste, but in the 1800s Aspdin and
Johnson discovered that when the entire batch was sintered and then ground, a superior cement was formed.
This substance became designated Portland cement (after the region in which they were working) and is the
most common cement in use today. Portland cement was first produced commercially in New Zealand in 1886
by James Wilson and Co., and has been produced here ever since. There are currently two companies
producing cement in New Zealand: Golden Bay Cement Ltd. in Whangarei and Milburn New Zealand Ltd. in
Westport. Production has increased from around 5000 t/annum in 1900 to in excess of 500 000 t/annum in 1991
and a New Zealand market demand in 1996 in excess of 800 000 t/annum. Portland cement is currently defined
as a mixture of argillaceous (i.e. clay-like) and calcaneus (i.e. containing CaCO3 or other insoluble calcium
salts) materials mixed with gypsum (CaSO4⋅2H2O) sintered and then pulverised into a fine powder. The precise
definition of Portland cement varies between different countries, and in New Zealand are controlled by New
Zealand's Standard Specification (NZS) 3122. Portland cement differs from its precursors primarily in the fact
that it is sintered.
Uses of Portland cement A summary of the uses of cement in New Zealand
is given in Figure 1. Cement is produced here in three main grades: ordinary
Portland cement (80% of Milburn's and 95% of Golden Bay's domestic
sales), rapid hardening cement and moderate-heat cement. Rapid-hardening
cement is used in precast concrete, pipes and tiles. It is finer ground so that
it hydrates more quickly and has more gypsum than other cements.
Moderate-heat cement is used for the construction of hydro-electric dams,
as the heat produced by ordinary cement creates uneven expansion and
hence cracking when such a large volume of concrete is used. In addition, a
few special cements are manufactured in New Zealand for larger projects or
export: these include sulphate resisting, flyash blend, blastfurnace slag and
Prise Mer cement.
THE MANUFACTURING PROCESS
Portland cement is made by heating raw materials rich in oxides of silicon,
calcium, aluminum and iron to temperatures of around 1200 - 1400o C. The
chemical reactions that occur within the partially molten mass result from the
formation of the four main cement materials.
Tricalcium silicate C3S 3CaO• SiO2 60-70
Dicalcium silicate C2S 2CaO• SiO2 10-20%
Tricalcium aluminate C3A 3CaO• Al2O3 5-10%
Tetracalcium alumino-ferrate C4AF 4CaO• Al2O3 •
Of these compounds, C3S and C3A are mainly responsible for the strength
of the cement. High percentages of C3S (low C2S) results in high early
strength but also high heat generation as the concrete sets. The reverse
combination of low C3S and high C2S develops strengths more slowly (over
52 rather than 28 days) and generates less heat. C3A causes undesirable
heat and rapid reacting properties, which can be prevented by adding
CaSO4 to the final product. C3A can be converted to the more desirable
C4AF by the addition of Fe2O3 before heating, but this also inhibits the
formation of C3S. C4AF makes the cement more resistant to seawater and
results in a somewhat slower reaction which evolves less heat. The balance
of the formed compounds versus the performance characteristics required
from the cement is a chemically controlled parameter. For this reason
considerable efforts are made during the manufacturing process to ensure
the correct chemical compounds in the correct ratios are present in the raw
materials before introduction of the materials to the kiln. The cement
manufacturing process involves four distinct stages, and these are outlined
Step 1 - Quarrying The raw material for cement manufacture is a rock mixture
which is about 80% limestone (which is rich in CaCO3) and 20% clay or shale (a
source of silica, alumina and Fe2O3). These are quarried and stored separately.
The lime and silica provide the main strength of the cement, while the iron
reduces the reaction temperature and gives the cement its characteristic grey
Step 2 - Raw material preparation The steps involved here depend on the
process used. There are two main cement manufacturing processes currently
used in New Zealand: the dry process (used by Golden Bay) and the wet process
(used by Milburn). The dry process uses more energy in grinding but less in the
kiln, and the wet process has lower overheads than the dry process. The two
processes are discussed separately below.
The dry process -The quarried clay and limestone are crushed separately until nothing bigger than a
tennis ball remains. Samples of both rocks are then sent off to the laboratory for mineral analysis. If
necessary, minerals are then added to either the clay or the limestone to ensure that the correct amounts
of aluminum, iron etc. are present. The clay and limestone are then fed.
together into a mill where the rock is ground until more than 85% of the material is less than 90µm in
The wet process- The clay is mixed to a paste in a washmill - a tank in which the clay is pulverised in the
presence of water. Crushed lime is then added and the whole mixture further ground. Any material which
is too coarse is extracted and reground. The slurry is then tested to ensure that it contains the correct
balance of minerals, and any extra ingredients blended in as necessary.
Step 3 - Clinkering This is the step which is characteristic of Portland cement. The finely ground material
is dried, heated (to enable the sintering reactions to take place) and then cooled down again. While it is
being heated various chemical reactions take place to form the major mineral constituents of Portland
The powder from the dry process doesn't contain much moisture, so can be dried
in a preheater tower. As it falls through the tower (which takes 30 seconds) it is
heated from 70 to 800o C. The moisture evaporates, up to 20% of the DE
carbonation (loss of CO2) occurs and some intermediate phases such as CaO•
Al2O3 begin to appear. The mixture is then fed into the kiln. The slurry from the
wet process contains too much moisture to be successfully dried in a preheater
tower. Instead, the slurry is fed directly into the kiln where it is formed into dry
balls by the heat and rotation of the kiln. Because of this extra role of the kiln, wet
process kilns are generally longer than dry process kilns: e.g. Milburn's kiln is
more than 100 m in length, whereas that used by Golden Bay is only 60 m long.
The kilns used in both processes are inclined on a shallow angle and lined with
The kiln- The kiln shell is steel, 60m long and inclined at an angle of 1 in 30.
The shell is supported on 3 roller trunions and weighs in at over 1100 T. The
kiln is heated by injecting pulverised coal dust into the discharge end where
it spontaneously ignites due to the very high temperatures. Coal is injected
with air into the kiln at a rate of 9 - 12 T hr-1. The reaction processes
occurring within the kiln are not easily understood due to the wide
variations in raw-mix chemistry, raw-mix physical properties and kiln
operating conditions, and the physical difficulties of extracting hot
materials from the process for investigation before they cool. Breaking the
reaction processes into a number of simple zones means we can make
some approximations about the cement formation process.
Zone 1: 0 - 35 min, 800 - 1100o C DE carbonation. Formation of 3CaO• Al2O3
above 900o C. Melting of fluxing compounds Al2O3 and Fe2O3. heat CaCO3 →
CaO + CO2
Zone 2: 35 - 40 min, 1100 - 1300o C Exothermic reactions and the formation of
secondary silicate phases as follows: heat 2CaO + SiO2 → 2CaO• SiO2
Zone 3: 40 - 50 min, 1300 - 1450 - 1300o C Sintering and reaction within the melt
to form ternary silicates and tetracalcium aluminoferrates: heat + time 2CaO•
SiO2 + CaO → 3CaO• SiO2 heat + time 3CaO• Al2O3 + CaO + Fe2O3 → 4CaO•
Al2O3 • Fe2O3
Zone 4: 50 - 60 min, 1300 - 1000o C Cooling and crystallisation of the various
mineral phases formed in the kiln.
The cooler Immediately following the kiln is a large cooler designed to drop the temperature of the clinker (as the
fused material is now called) from 1000o C to 150o C. This is achieved by forcing air through a bed of clinker via
perforated plates in the base of the cooler. The plates within the cooler slide back and forth, shuffling the clinker
down the cooler to the discharge point and transport to a storage area. At this point in the process the materials
have been formed into all the required minerals to make cement. Like cement, the clinker will react with water
and harden, but because it is composed of 1-3 cm diameter fragments it is too coarse to be used.
Step 4 - Cement milling To produce the final product the clinker is mixed with gypsum (CaSO4 • 2H2O), which is
added as a set retarder, and ground for approximately 30 minutes in large tube mills. The cement flows from the
inlet to the outlet of the mill (a rotating chamber), being first ground with 60 mm then 30 mm diameter steel balls.
The first grinding breaks up the material and the second grinds it to a fine powder. The amount of grinding is
governed by the volume of cement fed into the mill: the greater the volume the coarser the grind. This has
practical limits, with too much cement clogging up the mill and not enough actually increasing the particle size.
The particle size is measured by laser diffraction analysis, and the quantity of material entering the mill adjusted
accordingly. Over time the charge (steel grinding balls) wear out, so when they reach a certain size they fall
through a sieve and then are replaced. The cement grinding process is highly energy intensive. The largest mill
at Golden Bay Cement is some 11 m in length, weighs over 230 T, is driven by a 2100 kW motor and can produce
over 60 T hr-1. The rotating mill generates significant quantities of energy and water is added to both the inlet
and outlet ends of the mill to cool the product and the mill itself.